| ||Format||Pages||Price|| |
|5||$44.00||  ADD TO CART|
|Hardcopy (shipping and handling)||5||$44.00||  ADD TO CART|
This guide outlines the standard procedure for establishing and maintaining a preparatory cycle for electroplating on high carbon steel producing minimal hydrogen embrittlement and maximal adhesion of the electrodeposited metal. The reagents needed for this method are technical grade hydrochloric acid, nitric acid, sulfuric acid, and water. Steel substrates shall conform to required hardness, hydrogen embrittlement, and surface oxidation characteristics, and quality. Proper preplating treatments such as precleaning, stress relief treatment, mechanical treatment, electrolytic anodic cleaning, hydrochloric acid treatment, treatment for smut removal, anodic acid etching, and electropolishing shall be performed. Coating adhesion and embrittlement shall be tested.
This abstract is a brief summary of the referenced standard. It is informational only and not an official part of the standard; the full text of the standard itself must be referred to for its use and application. ASTM does not give any warranty express or implied or make any representation that the contents of this abstract are accurate, complete or up to date.
1.1 This guide is intended as an aid in establishing and maintaining a preparatory cycle for electroplating on high-carbon steel ( ) producing a minimum of hydrogen embrittlement and maximum adhesion of the electrodeposited metal. For the purpose of this guide, steels containing 0.35 % of carbon or more, and case-hardened low-carbon steel, are defined as high-carbon steels. There is no generally recognized definite carbon content dividing high from low-carbon steels for electroplating purposes.
Note 1: Electroplating of plain high-carbon steel introduced problems not found in similar operations on low-carbon steel. During the cleaning and electroplating cycle, high-carbon steel differs from low-carbon steel in regard to its greater tendency to become embrittled and the greater difficulty in obtaining maximum adhesion of the electrodeposit. The preparation of low-carbon steel for electroplating is covered in Practice .
1.2 This guide does not apply to the electroplating of alloy steel. For methods of chromium electroplating directly on steel see Guide .
1.3 The values stated in SI units are to be regarded as standard. No other units of measurement are included in this standard.
1.4 This standard does not purport to address all of the safety problems associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use. For a specific hazards statement, see .
ICS Number Code 25.220.20 (Surface treatment)
ASTM B242-99(2014)e1, Standard Guide for Preparation of High-Carbon Steel for Electroplating, ASTM International, West Conshohocken, PA, 2014, www.astm.orgBack to Top